Presentation on theme: "3.5 STRAIN ENERGY When material is deformed by external loading, energy is stored internally throughout its volume Internal energy is also referred to."— Presentation transcript:
13.5 STRAIN ENERGYWhen material is deformed by external loading, energy is stored internally throughout its volumeInternal energy is also referred to as strain energyStress develops a force,F = σ A = σ (x y)
23.5 STRAIN ENERGYStrain-energy density is strain energy per unit volume of materialu =∆U∆Vσ2=If material behavior is linear elastic, Hooke’s law applies,u =σ2σ22E=( )
33.5 STRAIN ENERGYModulus of resilienceWhen stress reaches proportional limit, strain-energy-energy density is called modulus of resilienceur =σpl pl2σpl22E=A material’s resilience represents its ability to absorb energy without any permanent damage
43.5 STRAIN ENERGYModulus of toughnessModulus of toughness ut, indicates the strain-energy density of material before it fracturesShaded area under stress-strain diagram is the modulus of toughnessUsed for designing members that may be accidentally overloadedHigher ut is preferable as distortion is noticeable before failure
5EXAMPLE 3.1Tension test for a steel alloy results in the stress-strain diagram below.Calculate the modulus of elasticity and the yield strength based on a 0.2%.
6EXAMPLE 3.1 (SOLN)Modulus of elasticityCalculate the slope of initial straight-line portion of the graph. Use magnified curve and scale shown in light blue, line extends from O to A, with coordinates ( mm, 345 MPa)E =345 MPamm/mm= 215 GPa
7EXAMPLE 3.1 (SOLN)Yield strengthAt 0.2% strain, extrapolate line (dashed) parallel to OA till it intersects stress-strain curve at A’σYS = 469 MPa
8EXAMPLE 3.1 (SOLN)Ultimate stressDefined at peak of graph, point B,σu = MPa
9EXAMPLE 3.1 (SOLN)Fracture stressWhen specimen strained to maximum of f = 0.23 mm/mm, fractures occur at C.Thus,σf = 621 MPa
103.6 POISSON’S RATIOWhen body subjected to axial tensile force, it elongates and contracts laterallySimilarly, it will contract and its sides expand laterally when subjected to an axial compressive force
113.6 POISSON’S RATIOStrains of the bar are:long =δLlat =δ’rEarly 1800s, S.D. Poisson realized that within elastic range, ration of the two strains is a constant value, since both are proportional.Poisson’s ratio, ν = −latlong
123.6 POISSON’S RATIOν is unique for homogenous and isotropic materialWhy negative sign? Longitudinal elongation cause lateral contraction (-ve strain) and vice versaLateral strain is the same in all lateral (radial) directionsPoisson’s ratio is dimensionless, 0 ≤ ν ≤ 0.5
13EXAMPLE 3.4Bar is made of A-36 steel and behaves elastically.Determine change in its length and change in dimensions of its cross section after load is applied.
14EXAMPLE 3.4 (SOLN)Normal stress in the bar isσz =PA= 16.0(106) PaFrom tables, Est = 200 GPa, strain in z-direction isz =σzEst= 80(10−6) mm/mmAxial elongation of the bar is,δz = zLz = [80(10−6)](1.5 m) = −25.6 μm/m
15EXAMPLE 3.4 (SOLN)Using νst = 0.32, contraction strains in both x and y directions arex = y = −νstz = −0.32[80(10−6)] = −25.6 μm/mThus changes in dimensions of cross-section areδx = xLx = −[25.6(10−6)](0.1 m) = −25.6 μmδy = yLy = −[25.6(10−6)](0.05 m) = −1.28 μm
163.6 SHEAR STRESS-STRAIN DIAGRAM Use thin-tube specimens and subject it to torsional loadingRecord measurements of applied torque and resulting angle of twist
173.6 SHEAR STRESS-STRAIN DIAGRAM Material will exhibit linear-elastic behavior till its proportional limit, τplStrain-hardening continues till it reaches ultimate shear stress, τuMaterial loses shear strength till it fractures, at stress of τf
183.6 SHEAR STRESS-STRAIN DIAGRAM Hooke’s law for shearτ = GγG is shear modulus of elasticity or modulus of rigidityG can be measured as slope of line on τ-γ diagram, G = τpl/ γplThe three material constants E, ν, and G is related byG =E2(1 + ν)
19EXAMPLE 3.5Specimen of titanium alloy tested in torsion & shear stress-strain diagram shown below.Determine shear modulus G, proportional limit, and ultimate shear stress.Also, determine the maximum distance d that the top of the block shown, could be displaced horizontally if material behaves elastically when acted upon by V. Find magnitude of V necessary to cause this displacement.
20EXAMPLE 3.5 (SOLN)Shear modulusObtained from the slope of the straight-line portion OA of the τ-γ diagram. Coordinates of A are (0.008 rad, 360 MPa)G == 45(103) MPa360 MPa0.008 rad
21EXAMPLE 3.5 (SOLN)Proportional limitBy inspection, graph ceases to be linear at point A, thus,τpl = 360 MPaUltimate stressFrom graph,τu = 504 MPa
22EXAMPLE 3.5 (SOLN)Maximum elastic displacement and shear forceBy inspection, graph ceases to be linear at point A, thus,tan (0.008 rad) ≈ rad =d50 mmd = 0.4 mmτavg =VA360 MPa =V(75 mm)(100 mm)V = 2700 kN
23*3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE Occurs when material supports a load for very long period of time, and continues to deform until a sudden fracture or usefulness is impairedIs only considered when metals and ceramics are used for structural members or mechanical parts subjected to high temperaturesOther materials (such as polymers & composites) are also affected by creep without influence of temperature
24*3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE Stress and/or temperature significantly affects the rate of creep of a materialCreep strength represents the highest initial stress the material can withstand during given time without causing specified creep strainSimple method to determine creep strengthTest several specimens simultaneouslyAt constant temperature, butEach specimen subjected to different axial stress
25*3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE Simple method to determine creep strengthMeasure time taken to produce allowable strain or rupture strain for each specimenPlot stress vs. strainCreep strength inversely proportional to temperature and applied stresses
26*3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE Defined as a metal subjected to repeated cycles of stress and strain, breaking down structurally, before fracturingNeeds to be accounted for in design of connecting rods (e.g. steam/gas turbine blades, connections/supports for bridges, railroad wheels/axles and parts subjected to cyclic loading)Fatigue occurs at a stress lesser than the material’s yield stress
27*3.7 FAILURE OF MATERIALS DUE TO CREEP & FATIGUE Also referred to as the endurance or fatigue limitMethod to get value of fatigueSubject series of specimens to specified stress and cycled to failurePlot stress (S) against number of cycles-to-failure N (S-N diagram) on logarithmic scale
28CHAPTER REVIEWTension test is the most important test for determining material strengths. Results of normal stress and normal strain can then be plotted.Many engineering materials behave in a linear-elastic manner, where stress is proportional to strain, defined by Hooke’s law, σ = E. E is the modulus of elasticity, and is measured from slope of a stress-strain diagramWhen material stressed beyond yield point, permanent deformation will occur.
29CHAPTER REVIEWStrain hardening causes further yielding of material with increasing stressAt ultimate stress, localized region on specimen begin to constrict, and starts “necking”. Fracture occurs.Ductile materials exhibit both plastic and elastic behavior. Ductility specified by permanent elongation to failure or by the permanent reduction in cross-sectional areaBrittle materials exhibit little or no yielding before failure
30CHAPTER REVIEWYield point for material can be increased by strain hardening, by applying load great enough to cause increase in stress causing yielding, then releasing the load. The larger stress produced becomes the new yield point for the materialDeformations of material under load causes strain energy to be stored. Strain energy per unit volume/strain energy density is equivalent to area under stress-strain curve.
31CHAPTER REVIEWThe area up to the yield point of stress-strain diagram is referred to as the modulus of resilienceThe entire area under the stress-strain diagram is referred to as the modulus of toughnessPoisson’s ratio (ν), a dimensionless property that measures the lateral strain to the longitudinal strain [0 ≤ ν ≤ 0.5]For shear stress vs. strain diagram: within elastic region, τ = Gγ, where G is the shearing modulus, found from the slope of the line within elastic region
32CHAPTER REVIEWG can also be obtained from the relationship of G = E/[2(1+ ν)]When materials are in service for long periods of time, creep and fatigue are important.Creep is the time rate of deformation, which occurs at high stress and/or high temperature. Design the material not to exceed a predetermined stress called the creep strength
33CHAPTER REVIEWFatigue occur when material undergoes a large number of cycles of loading. Will cause micro-cracks to occur and lead to brittle failure.Stress in material must not exceed specified endurance or fatigue limit